Determination of Young’sModulus by Specific Vibration of Basalt and Diabase

+e elasticity is an important parameter for the evaluation of the mechanical behavior of a rock mass and a fundamental factor in the definition of the resistance characteristics, stability, and blastability in rock blasts, and it is an important parameter for the blastability equations like the Kuz–Ram method. +is paper presents a comparison of the Uniaxial Compression Method (UCM) and the Impulse Excitation Technique (IET) in determining Young’s modulus. +e IET is a static and nondestructive dynamic method of characterizing mechanical parameters of materials, while the UCM is a quasistatic and destructive method. We determined Young’s modulus of samples from nine basalt and diabase mines used as aggregates in the construction industry. Young’s modulus was determined by the acoustic response due to longitudinal oscillations caused by a mechanical impulse (IET) in the Sonelastic equipment and the stress-strain curve (UCM). Young’s modulus values showed high repeatability and agreed with those reported in the literature for the same material. +e work shows that the solnelastic is an innovate equipment and elucidated advantages of IET in comparison to the UCM such as shorter execution time, greater safety, and a lower cost ranging from 11.5% to 22.5% of the UCM.


Introduction
e deformability is important for the evaluation of the mechanical behavior of a rocky massif [1] as it is a fundamental criterium for the definition of the resistance and blastability in rock blasts. Young's modulus and Poisson's coefficient characterize the mechanical behavior of a rock mass due to several simulation scenarios when applying tension variations and the use of explosives for blasting or fragmentation material in quarries. Young's modulus is one of the most important mechanical parameters for evaluating the mechanical stability of a material [2] used in established methods such as the Kuz-Ram and KCO models. e blastability index is the fragmentation capacity of a rock mass that is determined by the granulometric distribution of the blasted material, once the variables of the blast plane are defined. e Kuz-Ram method can be used to calculate the blastability index based on Young's modulus [3][4][5][6].
Young's modulus is influenced by characteristics of the rock such as discontinuities, petrographic structure, degree of weathering and alteration, void index and porosity, and elastic and plastic properties [1]. Static or quasistatic methods as the uniaxial and triaxial compression are commonly used to determine the abovementioned properties of materials. However, those methods are destructive, rendering the test pieces unusable [2].
Alternatively, the measurement of the natural frequency of a material using the forced resonant frequency can be used to determine dynamic Young's modulus, but this method is not routinely used in Brazil [7]. According to Bezerra [7], the stress-strain curve presents a nonlinear behavior for concrete, which hinders the accuracy of the values of static Young's modulus. e dynamic methods, which do not directly interfere in the sample because it does not exert tensions that cause changes in the physical behavior of the sample, provide more precise results. In addition, the use of dynamic Young's modulus is more appropriate to structures subjected to impact loads such as rock blast works.
Garaygordóbil [8] reported that the stress-strain curve does not present a linear behavior disturbing the calculation of a single value for Young's modulus; thus, nondestructive methods, which do not interfere directly with the sample, provide more accurate values. Carrasco et al. [9] found the IET to be a promising alternative for estimating Young's modulus of Brazilian wood. Only 2.46% of their predicted values were different of the estimated modules using a significance level of 95%. e IET principle is to measure the resonance frequencies by impulse indifferent vibrational modes: flexional, torsional, and longitudinal. ese vibrations are detected by an acoustic microphone and then converted to an electrical signal, recorded as a function of time. e signal is represented by the fast Fourrier transform as a function of the resonance frequencies of the sample. e elasticity constants of materials are calculated by the resonance frequency, density or mass, and dimensions of the sample [10]. e IET is a quick and effective method for measuring Young's modulus in undamaged samples [11]. Compared to the standard mechanical characterization, the IET is less affected by the typical heterogeneity of thick composite laminates and provides more repeatable results based on local strain measurements, but yields slightly larger values, probably because of the detrimental effect of the deformation rate [12]. e prediction of which resonances will be observed in a measurement is straightforward using the resonance eigenvalues and eigenvectors. A sinusoidal excitation is applied in some point on the sample, the response is measured in other point, and the process can be repeated for many frequencies [13]. Table 1 shows a comparison between quasistatic and dynamic methods [14]. erefore, the dynamic method presents advantages over the traditional quasistatic method because the determination is faster, it can be applied to several types of materials, the sample is not destroyed, the influence of the temperature in the elasticity can be determined, and it has less uncertainty especially when applied to determine the blastability of a rock [14]. e IET can also potentially be used to determine the modulus of dynamic elasticity in preventive maintenance and in the impact assessment of concrete structures that are subject to dynamic loads [15]. e IET is a dynamic method that uses the natural frequency of specific vibrations of each material [16] and characterizes Young's modulus and the damping by the acoustic response after a slight inserted mechanical impulse. Upon receiving a defined stimulation, the material generates elastic, transverse, and twisted longitudinal oscillations. When the yielded wavelength corresponds to the specific dimensions of the sample, there is a resonance effect with large amplitudes of oscillation [17]. e acoustic response is specific of each material and depends on the natural vibration frequencies of each material, which are proportional to Young's modulus and attenuation rate proportional to damping [16]. e time to obtain the natural frequency values is a fraction of a second. e acoustic response is picked up by a receiver in the opposite portion of the stimulus (1°- Figure 1), the acoustic response is converted in an amplitude graph (2°and 3°- Figure 1) by a specific software, and Young's modulus is determined (4°- Figure 1). e model for calculating Young's modulus from flexural vibration for circular section specimens is described below, according to ASTM E-1876 [18], E-1875 [19], and C215 [14,20].
where D is the diameter (mm), L the length (mm), m the mass (g), f f is the fundamental flexional resonance frequency, and T 1 is a correction factor for the fundamental flexion mode given by where μ is Poisson's ratio. e calculation of the uncertainty for Young's modulus in the flexional mode is given by

Advances in Materials Science and Engineering
If the L/D ratio ≥ 20, the correction factor T 1 ′ can be simplified to If the ratio L/D < 20 and Poisson's coefficient is known, then T 1 ′ can be calculated by equation 2. If L/D < 20 and Poisson's coefficient is unknown, then the iterative process shown should be used. e uniaxial compression method consists of assembling an upper and lower CAP sample set with lateral and axial extensometer, so the set is placed on the pedestal, and the load cell is approximate until the upper cap. en, a uniaxial load is applied at a constant loading or deformation rate, defined so that the loading time of the test is between 5 and 15 min. Unloading and loading can be performed to obtain the curves of stress-strain.
With the data, it is possible to calculate Young's modulus: where Δσ u a is the variation of uniaxial tension and Δε u a is the variation of deformation on generated line. e present work aims to compare IET and UCM to obtain Young's modulus of samples of a rock mass in terms of results, run time, sample preservation, safety, and costs.

Methods
e samples were randomly collected in five different quarries, EX, FV, and SA of basalt and NO and MG of diabase.
e specimens of rock were prepared for each quarry using a HILTI DD200 drill, with a 50 mm diameter. After sachets, each material was sawn to obtain cylindrical specimens with the length (L) ranging between 2 and 3 times the diameter (D), according to the American Society norms for Testing and Materials-ASTMD 2938-95 [21] and ASTM D4543-01 [22]. e specimens were dried in an electric oven for 4 h at 110°C and weighed. Table 2 shows the weight and density of the specimens. e elasticity modulus was determined by the IET in the Sonelastic equipment according to the norms of the International Society for Rock Mechanics (ISRM) [23], in the ATCP Engenharia Física, in Ribeirão Preto city. e equipment configuration was PC-based.
To perform the test, the nodal points were marked at a distance of 0.244 L from each end of the sample for support   Figure 2). e software was fed by the physical data depicted in Table 2 (mass, length, and diameter). Table 3 shows the technical characteristics of the acoustic microphone used.
After the preparation and positioning of the specimen, the values were measured in each sample. e data were then captured in the software, and the frequency spectrum was preprocessed.
rough the preprocessed spectrum, the process to obtain Young's modules was performed, choosing the largest amplitudes with care, so as to eliminate the harmonic peaks.
For uniaxial compression tests, the same samples as the IET test were used. e press used was a 2,000 kN EMIC DL3000 load capacity, with a dual configuration electric strain gauge, with independent sensors for measuring on either side of the specimen and equalizing box to obtain the average strain signal with a measuring range from 0.00001 to 2.50000 mm. e tests were performed in three loading and unloading steps up to 18 kN and then broken. Young's modulus values were obtained by the stress x strain curve generated by the UCM tests. Figure 3 shows the stress x strain curves for sample EX1, where UCM 1, UCM 2, and UCM 3 are, respectively, the charging 1, 2, and 3. e results of both tests were compared by Young's modulus values, costs, and test time between IET and UCM.  Table 4 assumes that the elasticity yielded by UCM is real, measuring how far the IET values are from the UCM ones. is error varied from 1 to 12%, indicating that the values yielded by the IET can represent Young's modulus of the analyzed samples.

Results and Discussion
An advantage of IET is the shorter run time of the assay. e average time interval between two measurements was   Advances in Materials Science and Engineering 6.5 min, which demonstrates the agility of the procedure, while for uniaxial compression, this average time is around 45 minutes (Table 4). Figure 4 shows the determined values of Young's modulus (E flex). e low values of standard deviation in the IET (<2.85 GPa) indicate that the measurements presents adequate repeatability. e IET measurements were much faster than a traditional measurement using the static method, which takes around 2 hours, since the interval between measurements was 6 ± 1.4 min.
Young's modulus of basalts and diabases ( Figure 4) agrees with those reported in the literature. For basalts, Aadnoy and Looyyeh (2014) found values ranging from 1.2 to 83.8 GPa and Caputo and Caputo [25] reported values of 100 GPa. For diabases, Lambe and Whitman [26] found values ranging from 86.87 to 116.52 GPa and Jaeger and Cook [27] reported values around 99.28 GPa.
Young's modulus of the EX, SA, and FV samples is very close and slightly differs from the values found for NO samples (Figure 4). ese discrepancies can be explained by the difference in the direction of the sample drawn, sampling at distinct points of the mine, and eventual presence of fractures in the specimen. Figure 5 shows the expected tendency of increase of Young's modulus (determined by both methods IET and UCM) as the density increases. Such relation has been reported for materials like bone [28], nanoporous self-assembled silicas [29], and self-sealed Si 3 N 4 /BN-based  Advances in Materials Science and Engineering 5 laminated structures [30]. Krstic and Krstic [30], for instance, found that any small decrease in the density of Si 3 N 4 / BN led to a large decrease in Young's modulus. e MG sample (density � 3.22 g/cm 3 ), however, does not follow this tendency, probably due to experimental differences during Young`s modulus determination. Table 5 shows the budgets elaborated between March 18 and 22, 2019, for flexural and/or longitudinal vibration IET tests compared to the standard uniaxial compression test. Vibration methods are cheaper than the compression method. In addition, there is little variation in the cost of determining Young's modulus by the vibration methods. e values presented in Table 5 show that for one to nine tests in the IET, the costs are about 22.5% of the UCM, and when the number of tests are higher than 10, these costs fall to 11.5%.
It must be emphasized that the execution of the tests through the IET method is safe because, since it is not destructive, there is no generation of fragments in the case of the rupture of the sample. e preservation of the test specimen is important for possible reproduction of the experiments and confirmation of the results. erefore, IET and the sonelastic are innovative promising techniques for the determination of Young's modulus of several materials, in comparison with the static method, since the execution of the measurement is faster, cheaper, and safer. e accuracy in determining Young's modulus is an advantage for the calculation of the blastability index, ensuring reliability to the evaluation of the mechanical behavior of a rock mass.

Conclusions
e IET method was suitable for the determination of Young's modulus since the found results presented high repeatability and agreed with those reported in the literature for the same type of materials. In addition, compared to UCM, the results were on average slightly higher (3.39%) for the IET, which is expected in a comparison between static and nonstatic testing. e costs for the IET analysis are about 11.5 to 22.5% of costs involved in the uniaxial compression method, depending the number of tests.
Because it is a nondestructive method, the IET is safer, with no risk of injury by throwing sample fragments and preserving them for future reevaluations. e time to perform IET testing is about 6.5 minutes, and UCM takes about 45 minutes or more, being about 6.9 times faster. e work highlighted important advantages of the IET in comparison with the traditional methods such as shorter execution time, higher safety, and nondestruction of the

Data Availability
ere are restrictions on data access because the work is still in progress.

Conflicts of Interest
ere are no conflicts of interest.